**Enhanced Performance GaAs-Based HBTs using a GaInNAs Base Layer **

K. S. Stevens, R. E. Welser, P. M. Deluca, B. E. Landini, C. R. Lutz, and T. L. Wolfsdorf-Brenner Kopin Corporation, 695 Myles Standish Boulevard, Taunton, MA 02780, USA

Phone: (508) 824-6696, Fax (508) 824-6418, E-mail: kstevens@kopin.com

**ABSTRACT**

**GaInNAs base layers are enabling performance **
**enhancements over standard GaAs-based HBTs, while **
**preserving the cost effective GaAs platform. We have **
**demonstrated InGaP/GaInNAs HBTs which offer **
**115 mV lower operating voltage, improved diode **
**symmetry for reduced VCE,offset and Vknee, and superior **

**gain temperature stability as compared with standard **
**InGaP/GaAs HBTs. These enhancements have been **
**realized while simultaneously preserving DC current **
**gain and base doping (ββββ ∼∼∼∼ 80, Rsb** **∼∼∼∼ 530 Ω/**Ω/Ω/Ω/**, base **

**thickness ∼∼∼∼ 500 Å, base doping ~ 4××××1019 _{ cm}2_{) at the }**

**high levels necessary for commercial applications. **
**GaInNAs enables these performance enhancements **
**due to a lower energy gap which advantageously alters **
**relative magnitudes of the collector and various base **
**current components in an HBT. **

INTRODUCTION

GaAs-based heterojunction bipolar transistor (HBT) integrated circuits have developed into a key technology for a variety of applications, particularly as power amplifiers for wireless handsets and high speed (>10 Gbit/s) circuits for fiber optic communication systems. However, there is ever increasing demand for performance enhancements to the basic GaAs-based HBT. Increased handset circuit complexity, higher efficiency and lower power dissipation for extended battery lifetime, faster fiber optic bit rates, and improved robustness are some of the motivating issues. The relevant device performance enhancements include lower minimum operating voltage, improved gain stability, greater reliability at increased current densities, lower VCE,offset and Vknee, and shorter

transit times. Manipulating the relative magnitudes of the collector and various base current components in a GaAs-based HBT will help realize most all these improvements.

To first order, there are five current components for state of the art GaAs-based HBTs operating in active mode. One

component describes the collector current (IC)

and the other four comprise the base current (IB). The collector current is simply the

base-emitter forward biased diode diffusion current, which is exponentially dependent on the base-emitter voltage (Vbe). The base current is

composed of space charge recombination (ISC),

neutral base recombination (INB), reverse hole

injection (IRHI), and surface recombination (ISR)

currents. By manipulating these currents, several device enhancements can be realized. Increasing IC for fixed Vbe lowers the operating

voltage of the HBT. This also reduces the relative contribution of ISC, ISR and IRHI to IB,

thereby improving gain stability and reliability [1,2]. Matching current for the base-emitter and base-collector junctions at the same forward bias (Vbe and Vbc, respectively), minimizes the

offset voltage (VCE,offset) and knee voltage

(Vknee). These reductions should allow for

improved PAE [3,4].

The current component adjustments described above can be achieved by lowering the base layer energy gap (Eg,b), while taking

care to minimize the impact of conduction band spikes. These adjustments, in turn, result in device performance enhancements. To achieve this, while at the same time preserving the cost effective GaAs platform, we substitute p+-GaInNAs for p+-GaAs as the HBT base layer. Numerous laboratories have demonstrated that the energy-gap of GaInAs decreases substantially when small amounts of N are incorporated into the material [5,6]. More importantly, GaInNAs alloys can be grown lattice-matched to GaAs because In and N have opposing strain effects on the lattice (N adds tensile strain, In compressive). Using this quaternary system, it should also be possible to engineer a strain-free graded Eg base layer,

thereby enhancing the frequency performance of the device. The bandgap engineering enabled

by GaInNAs is being aggressively developed for a variety of device applications, including laser diodes, multijunction solar cells, HBTs and HEMTs [5-10]. In this report, we present our current results for exploiting the GaInNAs material system to enhance the performance of GaAs-based HBTs.

EXPERIMENT

The basic InGaP/GaInAsN DHBT device structures explored in this work are identical to standard InGaP/GaAs HBTs except for the addition of In and N to the base layer, as described elsewhere [9]. All samples have MOCVD-grown, C-doped base layers varying between 1.5-6x1019 cm-3 in doping and 500-1500 Å in thickness, resulting in Rsb values

between 100 and 850 Ω/. The electrical and structural properties of the GaInAsN base layer are determined directly from the InGaP/GaInAsN DHBT structure by a combination of transistor measurements, Polaron C-V profiles, photoluminescence (PL) signals, and double crystal x-ray diffraction spectrum [11]. Large area devices (L = 75 µm x 75 µm) are fabricated using a simple wet-etching process and tested in the common base and common emitter configurations.

RESULTS AND DISCUSSION

Our basic approach for developing InGaP/GaInAsN DHBTs is iterative in nature and focuses on obtaining both high p-type base doping levels and acceptable dc current gain characteristics. Using standard 4x1019 cm-3 p-type GaAs base layers as a base line, we add small amounts of In and N, optimize the growth for maximum doping and dc current gain, and then incrementally increase both the In and N levels, thereby lowering Eg,b. Separate sets (e.g.

A through F) of InGaP/GaInNAs DHBTs are thus defined as having different Eg,b.

Using the GaInNAs base layer approach, we have achieved turn-on voltage reductions up to 115 mV relative to other GaAs-based bipolar structures. This is illustrated in Figure 1, which shows the Vbe required to achieve a certain fixed

collector current density (JC) as a function of

base sheet resistance (Rsb). Standard

InGaP/GaAs HBTs and GaAs/GaAs BJT data are included to establish the fundamental lower limit of the turn-on voltage that can be achieved using a GaAs base layer [9]. To help quantify turn-on voltage reductions, a solid line is included and indicates a logarithmic fit to this data. Three sets of InGaP/GaInNAs DHBT data are fitted by the same logarithmic dependence on Rsb, allowing for a Vbe shift due to bandgap

narrowing. These fits show 45, 80, and 115 mV reductions in turn-on voltage for the three sets of InGaP/GaInNAs DHBTs. Comparison of JC

vs. Vbe shows this turn-on reduction is

maintained for over five decades of current, corresponding to a two order of magnitude increase in JC for a fixed Vbe.

y = -0.0177Ln(x) + 1.194
R2_{ = 0.9248}
0.945
0.965
0.985
1.005
1.025
1.045
1.065
1.085
1.105
1.125
50 150 250 350 450 550 650 750 850

**Base Sheet Resistance (**ΩΩΩ**Ω/****)**
**Vbe**
** @**
** 1.**
**78A**
**/c**
**m**
**2**
InGaP/GaInAsN DHBTs
InGaP/GaAs HBTs
BJTs (GaAs/GaAs)
Set C:
∆Vbe = - 45.0 mV
Set E:
∆Vbe = - 80.0 mV
Set F:
∆Vbe = - 115.0
mV

Fig. 1. Turn-on Vbe (@ JC = 1.78A/cm2) as a function of

Rsb for standard InGaP/GaAs HBTs and GaAs/GaAs

BJTs. Also shown are data for 3 sets of InGaP/GaInNAs DHBTs, sets C, E, and F, each with different ∆Vbe. The

solid line represents a logarithmic fit to the InGaP/GaAs HBT data. The dashed lines represent 45.0, 80.0 and 115.0 mV reductions to the same logarithmic fit and are used as a guide for the eye.

Increased IC for a given Vbe lessens the

asymmetry of the base-emitter / base-collector diode pair. For the wide bandgap InGaP emitter HBTs under consideration here (no conduction band spikes), IBEF is dominated by the diffusion

current (n = 1) exponential term which is highly sensitive to Eg,b. However, the forward biased

base-collector diode current (IBCF) is dominated

by the recombination current (n = 2) exponential term which is governed largely by the collector properties and is insensitive to the heavily doped base layer properties, including Eg,b [4]. The net

result is that lowering Eg,b using p+ GaInNAs,

improves the symmetry of the base-emitter / base-collector diode pair of the HBT. This should lower VCE,offset (and by extension Vknee)

since its value is related to the difference between Vbe and Vbc where IBEF = IBCF [4].

Figure 2 shows the base-emitter (IBEF) and

base-collector (IBCF) currents as a function of

diode forward bias for a large area (75 µm x 75 µm) InGaP/GaInNAs (set E) DHBT and a standard InGaP/GaAs HBT. As expected, the InGaP/GaInNAs HBT data show reduced Vbe - Vbc difference for fixed forward biased

diode current.
1.0E-10
1.0E-09
1.0E-08
1.0E-07
1.0E-06
1.0E-05
1.0E-04
1.0E-03
1.0E-02
1.0E-01
-1.3
-1.2
-1.1
-1
-0.9
-0.8
-0.7
-0.6
-0.5
**Forward Bias (V)**
**Fo**
**rw**
**ar**
**d**
** C**
**u**
**rr**
**e**
**n**
**t (A**
**)**
InGaP/GaAs HBT
InGaP/GaInAsN DHBT
**IBEF (n~1)**
**IBCF (n~2)**
**Vce,offset ~ Vbe – Vbc **
**@ fixed I**

Fig. 2. Base-emitter (IBEF) and base-collector (IBCF)

currents as a function of diode forward bias for a large area (75 µm x 75 µm) InGaP/GaInNAs (set E) DHBT and a standard InGaP/GaAs HBT.

Figure 3 shows the common emitter characteristics for a large area InGaP/GaInNAs DHBT exhibiting VCE,offset ~ 100 mV. This is

slightly lower than we typically obtain for InGaP/GaAs HBTs. It should be noted that an unoptimized device geometry contributes significantly to VCE,offset of these devices. The

base-collector interface must be well engineered due to the presence of a conduction band discontinuity between the p+ GaInNAs base and n –GaAs collector. The high output impedance of this InGaP/GaInNAs HBT (Fig. 3) indicates the lack of a conduction band spike at the base-collector interface.

The data presented above demonstrate properly engineered InGaP/GaInNAs (lower Eg,b) HBTs give increased IC for a given Vbe, as

compared to InGaP/GaAs HBTs. Reduced Eg,b

and increased IC (through a corresponding

increase of INB) reduce the relative contribution

of ISC, ISR and IRHI to IB [1,2]. Since IRHI is

extremely temperature sensitive, reducing its contribution to IB should improve gain

temperature stability of the device [12,13].

-1.0E-02
0.0E+00
1.0E-02
2.0E-02
3.0E-02
4.0E-02
5.0E-02
6.0E-02
7.0E-02
8.0E-02
9.0E-02
0 1 2 3 4 5 6
**Vce (V)**
**Ic**
** (A**
**)**

InGaP/GaInAsN DHBT (Set E), ∆Ib = 228 µA

VCE,offset ~ 100 mV

Fig. 3. Common emitter characteristics for a large area
(75 µm x 75 µm) InGaP/GaInNAs (set E) DHBT
(VCE,offset ~ 100 mV).
0
10
20
30
40
50
60
70
80
90
100
110
120
130
140
150
160
170
180
190
200
-20 0 20 40 60 80 100 120
**Temperature (o _{C)}**

**DC Current Gain**

**ββββ @ 1.78 kA/cm2**InGaP/GaAs HBT InGaP/GaInAsN DHBT 25% AlGaAs/GaAs HBT

Fig. 4. DC Current gain (β) as a function of temperature for a 25%AlGaAs/GaAs HBT, an InGaP/GaAs HBT, and an InGaP/GaInNAs (∆Vbe = -100 mV, Rsb ~ 530 Ω/,

thickbase = 500 Å) DHBT.

Figure 4 shows DC current gain as a function of temperature which illustrates the superior gain temperature stability of InGaP/GaInNAs HBTs as compared to InGaP/GaAs and 25%AlGaAs/GaAs HBTs. InGaP/GaAs HBTs exhibit superior gain temperature stability compared to 25%AlGaAs/GaAs HBTs due to the larger hole barrier. The larger hole barrier is a result of the larger band gap of InGaP as compared to 25%AlGaAs [13]. This hole barrier is increased further via the reduced Eg,b

of GaInNAs as compared to GaAs. Additionally, the temperature dependence of the

minority carrier lifetime in the GaInNAs base may be less than for a GaAs base [7]. For the InGaP/GaInNAs HBTs, these two mechanisms likely explain the absence of DC current gain temperature dependence over all current densities and temperatures measured in this study (Fig. 5). 0 10 20 30 40 50 60 70 80 90

1.0E-08 1.0E-07 1.0E-06 1.0E-05 1.0E-04 1.0E-03 1.0E-02 1.0E-01 1.0E+00 1.0E+01
**Current Density (kA/cm2 _{)}**

**DC Current Gain**
0 oC
20oC
40oC
60oC
80oC
100oC

Fig. 5. DC Current gain (β) as a function of current density for an InGaP/GaInNAs (∆Vbe = -100 mV, Rsb ~

530 Ω/, thickbase = 500 Å) DHBT for a range of

temperatures. CONCLUSIONS

Performance enhancements to the standard GaAs-based HBT are feasible through alterations to the relative magnitudes of the collector and various base current components. GaInNAs base layers allow these current manipulations and realize these sought after improvements through reducing Eg,b. To date,

we have demonstrated InGaP/GaInNAs HBTs which offer 115 mV lower operating voltage, improved diode symmetry for reduced VCE,offset

and Vknee, and superior gain temperature

stability as compared with standard InGaP/GaAs HBTs. These enhancements have been realized while simultaneously preserving DC current gains and base doping levels (β ∼ 80, Rsb ∼

530 Ω/, base thickness ∼ 500 Å, base doping
~ 4×1019_{ cm}2_{) which are useful for practical }

applications. Significant improvements in these and other performance enhancements are expected as growth of this new material system matures.

REFERENCES

[1] T. S. Low, C. P. Hutchinson, P. C. Canfield, T. S. Shirley,

R. E. Yeats, J. S. C. Chang, G. K. Essilfile, M. K. Culver, W. C. Whiteley, D. C. D’Avanzo, N. Pan, J. Elliot, C. Lutz; Migration from an AlGaAs to an InGaP Emitter HBT IC Process for Improved Reliability; 1998; GaAs IC Symp.; 153-156.

[2] R. E. Welser, M. Chaplin, C. R. Lutz, N. Pan; Base Current Investigation of the Long-Term Reliability of GaAs-Based HBTs; 2000; GaAs MANTECH; 145-148.

*[3] N. Bovolon et al., Theoretical and Experimental *
Investigation of the Collector-Emitter Offset Voltage of
AlGaAs/GaAs Heterojunction Bipolar Transistors; 1999; IEEE
Trans. Electron Devices; 46; 622-627.

[4] K. Mochizuki, R. J. Welty, P. M. Asbeck, C. R. Lutz, R. E. Welser, S. J. Whitney, and N. Pan; GaInP/GaAs Collector-Up Tunneling-Collector Heterojunction Bipolar Transistors (C-Up TC-HBTs): Optimization of Fabrication Process and Epitaxial Layer Structure for High-Efficiency High-Power Amplifiers; 2000; IEEE Trans. Electron Devices; 47; 2276-2283.

[5] K. Nakahara, K. Kondow T. Kitatani, Y. Yazawa, and K. Uomi; Continuous-wave operation of long-wavelength GaInNAs/GaAs quantum well laser; 1996; Electon. Lett.; 32; 1585.

[6] S. R. Kurtz, A. A. Allerman, E. D. Jones, J. M. Gee, J. J. Banas, and B. E. Hammons; InGaAsN solar cells with 1.0 eV band gap, lattice matched to GaAs; 1999; Appl. Phys. Lett; 74; 729.

[7] R. J. Welty, H. P. Xin, K. Mochizuki, C. W. Tu, and P. M. Asbeck; Design and Characterization of GaAs/

Ga0.89In0.11N0.02As0.98/GaAs NpN Double Heterojunction Bipolar

Transistors with Low Turn-on Voltage; 2000; Proc. of the Device Research Conference; 145-146.

[8] P. C. Chang, A. G. Baca, N. Y. Li, X. M. Xie, H. Q. Hou, and E. Armour; InGaP/InGaAsN/GaAs NpN double-heterojunction bipolar transistor; 2000; Appl. Phys. Lett; 76; 2262-2264.

[9] R. E. Welser, P. M. DeLuca, and N. Pan; Turn-on Voltage

Investigation of GaAs-based Bipolar Transistors with Ga

1-xInxAs1-yNy Base Layers; 2000; IEEE Elec. Dev. Lett.; 21;

554-556.

[10] T. Kikkawa, K. Makiyama, T. Nishioka, and H. Tanaka; High Electron Mobility Transistor using GaInAsN Channel Grown by LP-MOVPE; 2000; Electronic Materials Conference. Denver.

[11] R. E. Welser, P. M. DeLuca, A. C. Wang, and N. Pan; Low

Vbe GaInAsN Base Heterojunction Bipolar Transistors; 2000;

TWHM ’00.

[12] C.-M. S. Ng, P. A. Houston, H.-K. Yow; Analysis of the Temperature Dependence of Current Gain in Heterojunction Bipolar Transistors; 1997; IEEE Trans. Electron Devices; 44; 17-24.

[13] R. E. Welser, N. Pan, C. R. Lutz, D. P. Vu, P. J. Zampardi, R. L. Pierson, B. T. McDermott; High Performance

Al0.35Ga0.65As/GaAs HBT’s; 2000; IEEE Electron Device Lett.;